Piezoelectric and ferroelectric properties of KNN.
Ferroelectric ceramics were discovered in the 1940s in polycrystalline barium titanate (von Hippel et al., 1946; Wul & Goldman, 1945), since then, there has been a continuous succession of new materials and technology developments that have led to a significant number of industrial and commercial applications.
Structurally speaking there are four types of ferroelectric ceramics: (1)perovskites, (2) the tungsten-bronze group, (3) pyrochlores and (4) the bismuth layer-structure group. Of these, the perovskites (ABO3) are by far the most important category. The families with composition BaTiO3, PbZr1-xTixO3 (PZT), PZT:La (PLZT), PbTiO3(PT), Pb(Mg1/3Nb2/3)O3(PMN) and (K0.5Na0.5)NbO3(KNN) represents most of the ferroelectric ceramics manufactured in the world (Haertling, 1999).
In this chapter the structure of calcium titanium oxide (CaTiO3), the ferroelectrics ceramics BaTiO3,Na0.5Bi0.5TiO3 (NBT), K0.5Bi0.5TiO3 (KBT) are described as well the concept of hysteresis loop, ferroelectric domains and why lead free materials are now in the top of the interest in ferroelectric and piezoelectric materials. The aim of this chapter is to present results of the synthesis, characterization and piezoelectric properties of two lead free piezoelectric compounds: K0.5Na0.5NbO3 and (K0.48Na0.52)0.96Li0.04Nb0.85Ta0.15O3.
1.1. Perovskite structure
The mineral perovskite is calcium titanate, with chemical formula CaTiO3, its ideal structure has space group
The perovskite type structure is enormously tolerant to variations in composition and distortions due to its ability to adapt a mismatch between the equilibrium A-O and B-O bond lengths, allowing the existence of a large number and variety of stoichiometric compounds. Those distortions, for instance tetragonal (Fig. 2), orthorhombic, rhombohedral and monoclinic, give rise to changes in the crystal symmetry, and one or more cations shift from high-symmetry positions in the lattice, producing ferroelectric or antiferroelectric behavior. In other words, the center of positive and negative charge within the unit cell is no longer coincident, which is the origin of the spontaneous polarization. However, in a ferroelectric material the spontaneous polarization is necessary but not sufficient, since it also requires the reorientation of the polarization by an electric field.
2. Some characteristics of ferroelectric materials
2.1. Hysteresis loop: the fingerprint of ferroelectricity
As mentioned-above, a distinctive feature of ferroelectricity is the reorientation of the polarization by an electric field. Thus, the observation of some evidence of switching is fundamental to establish the ferroelectricity. The experimental evidence is given by the electric hysteresis loop; actually, the term ferroelectric was coined in analogy with the similar magnetic loop
2.2. Ferroelectric domains
The volume regions of the material with the same polarization orientation are referred to as ferroelectric domains. When the sample is under zero field and strain-free conditions, all the domain states have the same energy; but if an electric field is applied, the free energy of the system is lowered by aligning the polarization along the field. Thus, large applied electric fields can permanently reorient the polarization between the allowed domain states, which are restricted by crystallography. As a result, even ceramics, constituted by polycrystals randomly oriented can be electrically poled to produce net piezoelectric coefficients. Much of the importance of ferroelectric materials is due to their properties, leading to a wide range of applications. Among these applications are high dielectric constant capacitors, piezoelectric sonar, ultrasonic transducers, ultrasonic motors, actuators and pyroelectric detectors. Special mention is reserved for the ferroelectric memories, field effect and cooling devices.
2.3. A way to improve the electromechanical properties of ferroelectric ceramics: morphotropic phase boundary (MPB) and polymorphic phase transition (PPT)
In analogy to the characteristics of the PZT (PbZr1-xTixO3) phase diagram, which presents a MPB between tetragonal and trigonal phases (Jaffe, 1971) (which means literally
2.4. The environmental issue: lead-free based materials
The most widely used ferroelectric ceramics are those based on the PbTiO3–PbZrO3 solid solution, generically called PZT. The PZT is composed of about 60 wt.% of lead, which rises ecological concerns; thus, some countries have legislated to replace this material by lead-free ceramics (European commission, 2008) since lead is a toxic element that affects the human health and the environment. Consequently, in recent years diverse systems are being investigated, among them, barium titanate (Yoon et al., 2007), bismuth-alkaline metal titanates and niobates (Hao et al., 2005; Jing et al. 2003; Ma et al., 2006), especially the K0.5Na0.5NbO3 solid solution abbreviated KNN (Du et al., 2006; Saito et al., 2004).
3. Important lead-free ferroelectric ceramics with perovskite structure
The first oxide with perovskite-type structure exhibiting ferroelectric behavior was BaTiO3 (BTO) (von Hippel et al., 1946; Wul & Goldman, 1945). It played a major role in demonstrating that ferroelectric ceramics had piezoelectric response through the poling process. At these days, the prevailing opinion was that ceramics could not be piezoelectrically active, because the randomly oriented dipoles would, on the whole, cancel out each other. This was proved not to be true for ferroelectrics ceramics, in which the dipoles could be permanently aligned or reoriented with an electric field. One of the fundamental issues in the understanding of ferroelectricity and piezoelectricity in ceramics was the discovery of the unusually high dielectric constant of BTO (Jaffe, 1958). Although BTO does not exhibit high piezoelectric constants, it has high relative permittivity. For this reason, BTO is the most widely used material in capacitors. Billions of BTO condensers are still made annually, at a cost of less than one cent per capacitor (Scott, 2007). However, BTO has an important drawback, its relatively low Curie temperature (~120 °C) (Merz, 1949). While advances in order to improve the piezoelectric properties and to increase the Curie temperature are concurrently underway, they have had little success. The observation of large and colossal permittivity (104-106) (West, 2006, Yu et al., 2004) in the BTO, has consolidate it as a material for capacitors. For instance, (Ba0.92Ca0.08)(Ti0.95Zr0.05)O3 has high piezoelectric coefficient
3.2. Na0.5Bi0.5TiO3 and K0.5Bi0.5TiO3
Bismuth sodium titanate Na0.5Bi0.5TiO3 (BNT), was discovered 50 years ago (Smolenskii et al., 1961), it shows strong ferroelectric properties with a significantly remnant polarization of 38 μC/cm2, and a Curie temperature of 320°C. However, this ceramic has disadvantages such as high conductivity and large coercive field (~73 kV/cm), which cause problems in the poling process. Data on exact piezoelectric properties of the BNT ceramic are insufficient due to the as-mentioned difficulties at the poling process. On the other hand, the BNT ceramic needs a high sintering temperature (>1200°C) to obtain dense samples. It is thought that the vaporization of Bi+3 ions occurred during the sintering process at temperatures higher than 1200°C, resulting in the poor poling treatments because of the high conductivity. As in the case of BTO, there have been efforts to improve the piezoelectric response of NBT by the substitution of one or more of its ions. Different authors have studied solid solutions of NBT with BTO, K0.5Bi0.5TiO3 (Takenaka et al., 2008) and KNN (Nagata et al., 2003; Yao et al., 2009; Zhang 2008). All these attempts try to exploit the morphotropic or polymorphic phase boundaries, where it is known that an improvement of dielectric and piezoelectric properties exist. In addition, some rare earths such as La, Y, Ce and some transition metals such as Co, Nb and Mn (Li et al., 2004; Nagata & Takenaka, 2001; Takenaka et al., 1990; Zhou et al., 2009) have been used. Some results are promising, but still more work is needed to improve the dielectric and piezoelectric properties simultaneously.
Just as the NBT, the KBT was discovered 50 years ago (Smolenskii et al., 1961). KBT has tetragonal symmetry at room temperature and a relatively high
3.3. K0.5N0.5NbO3 (KNN)
The pioneering work on KNbO3-NaNbO3solid solution was carried out in the mid-50s of last century (Shirane et al., 1954). KNN is a specific composition on a complete solid solution of antiferroelectric NaNbO3 and ferroelectric KNbO3, namely, 50:50. This composition is close to the MPB between two orthorhombic phases, resembling the PZT system. Undoubtedly, the KNN and the derived compounds are the most promising lead-free ferroelectric materials demonstrated by the results published some years ago (Saito et al., 2004). The major contribution of this work was to show the modification of the PPT, present in KNN (Shirane et al., 1954), by the addition of Li+1 and Ta+5. Since then, this system has been caused a lot of interest and many studies have been done onthis field. In fact, our research deals with this material which is presented in section 6. The main obstacles in the processing of KNN are the synthesis and sinteringsteps that will be treated in next two sections. These difficulties occur, since the alkaline elements undergo sublimation at the high temperature required to achieve the adequate densification, which changes the initial stoichiometry considerably. This problem has been addressed through different methods, one of these involves densification improvement by the addition of some oxides such as CuO, MnO2, CeO2 (Gao et al., 2009; Yang et al., 2010; Yin et al., 2010). According to these researches, it is believed that these compounds form a liquid phase at low temperature, thus promoting densification. Another approach involves addition of A and B elements into the ABO3 structure of the KNN solid solution. In the A site, several cations can be added, e. g. Li+, Ba2+, La3+, Bi3+, whereas for the B site it is possible to introduce Ti4+, Sb5+ or Ta5+ (Ahn et al., 2009; Hagh et al., 2009; Jiang et al., 2009). The ion substitution can induce phase transformation and consequently a better performance of materials. A third way to improve densification is by reducing the particle size of the synthesized powders; however, since the conventional ceramic method does not achieve considerable reduction of particle size, then, the sol–gel, Pechini and hydrothermal methods have been used. Furthermore, the chemical homogeneity of the KNN compound with Li+1 and Ta+5 dopants synthesized by the conventional solid state reaction route has revealed an inhomogeneous distribution of Nb5+, Ta5+, K+ and Na+ cations, which leads to a considerable detriment of the piezoelectric properties, being one reason for the discrepancy among the data reported by several authors for the same or similar composition (Y. Wang et al., 2007). All these issues are addressed in the subsequent sections, which are the central part of our contribution.
4. Synthesis of KNN and co-doped KNN
This section will be dedicated to briefly review some methods used for the synthesis of KNN and related compositions. The ceramic method is discussed first, and then the chemically methods used in an effort to obtain chemical homogeneous powders. These include the sol-gel, Pechini and hydrothermal methods. They have produced some interesting results, but there are still some issues that must have the attention of the researchers.
4.1. Conventional ceramic method
For the synthesis of KNN lead-free ferroelectrics, the initial point is the ceramic method (CM), this is the simplest method for the production of ceramic materials. The conventional method is well-known and extensively used, and was the first method reported for the synthesis of KNN (Egerton & Dillon, 1959; Jaeger & Egerton, 1962; Shirane et al., 1954), since it is simple and low cost. Basically, it consists of mixing carbonates and oxide powders of the desired elements. The process is carried out in a conventional ball mill, or in mills that supply more energy as the attrition or planetary ball mills (high energy mills), with the purpose to obtain a homogeneous mixture of the powders. The process is performed in liquid media for a better mixing; the most popular liquids are absolute ethanol and acetone, the former being cheaper and with low toxicity. During grinding, the powders undergo grain size reduction, and become amorphous if high energy milling is used. Once the mixture is ready, this is calcined at an adequate temperature, which depends on composition. In the case of the lead-free ceramics based in KNN, these temperatures are between 800 and 950° C. The heat treatment should be carried out for several hours. Finally, the crystalline powders are grinded again to reduce the particle size for their subsequent pressing and sintering. The advantages of this method are the inexpensive equipment and low costof reagents. On the other hand, high temperature calcinations and long time of the heat treatments usually results in considerable loss of alkaline elements; furthermore, two steps of grinding are also needed.
4.2. The sol-gel method
Taking into account the characteristics of the powders obtained by means of the conventional method, the so-called chemical routes have been investigated for the synthesis of lead-free ferroelectric ceramic powders. Among them, the sol-gel method (Shiratori et al., 2005; Chowdhury et al., 2010) has been reported to produce KNN nanometric powders. The technique consists of mixing metal-organic compounds (mainly alkoxides) in an organic solvent, the subsequent addition of water generates two reactions, hydrolysis and polymerization, producing the gel which is dried and calcined for obtaining crystalline ceramics. The method has some advantages, such as the nanometric and chemical homogeneity of the powders and the low crystallization temperature (Shiratori et al., 2005). The disadvantages of this procedure are the utilization of metal-organic chemicals, which are expensive. Besides, they need of a strict control of the conditions for the reaction since they generally possess a different hydrolysis rate and must be handled under free moisture atmosphere for avoiding the rapid decomposition of alkoxides. The addition of organic compounds is necessary to improve the dispersion and to obtain fine powders.
4.3. Pechini method
One of the chemical methods that have attracted attention in the synthesis of ceramic materials is the Pechini method. The process implies the formation of a polymeric resin between an organic acid and an alcohol (generally ethylene-glycol). The precursor solution should be heated to evaporate the solvent and to promote the formation of the resin. Once the resin is obtained, it is crushed and calcined at different temperatures to observe the crystallization evolution. As in the case of sol-gel, the Pechini route also uses niobium moisture sensitive reagents, so that the problems are similar in both methods. Despite these drawbacks, the very fine powders obtained are promising to produce dense ceramics, but there are not reports on the piezoelectric properties of ceramics synthesized by this method, only the synthesis of KNN powders is reported (Chowdhury et al., 2009). In this study the authors used an ammonium niobate oxalate hydrate instead the alkoxide. With this approach nanometric powders were synthesized.
4.4. Hydrothermal method
With the aim to obtain KNN ceramic powders at low temperature andto avoid the loss of sodium and potassium, the hydrothermal method have been used recently (Sun et al., 2007; Maeda et al., 2010; N. Liu, et al., 2009 ). This method involves placing the reagents into a pressurized reactor or autoclave, the reaction is carried out at low temperature (< 300°C) where the pressure generated depends on the temperature at which the reactor is heated. The studies reported until now suggest a processing time of 6-24 hours at the desired temperature. Nevertheless, these studies also indicate that the resultant products are composed of two phases, a sodium rich phase and another with greater quantity of potassium. The reagents that have been used in these experiments are potassium and sodium hydroxides, whit a KOH/NaOH molar ratio between 3/1 and 4/1, and the total concentration around 6 M of hydroxides. Alternatively, the synthesis of KNN has also been reported by means of the microwave-hydrothermal method at 160°C for 7 hours with an alkalinity of 6 M (Zhou et al., 2010) the authors underline that improved piezoelectric constant
As a final comment for this synthesis section, it is important to mention that the powder characteristics obtained by any synthesis method may aid the sintering stage, therefore the powders should be chemically pure i.e. without secondary phases, the calcination temperature (except in hydrothermal synthesis) must be as low as possible to avoid the considerable loss of alkaline compounds, and the nanometric powders are more suitable since thesecontribute to an additional driving force for sintering.
5. Sintering of KNN and related compositions
Just like the synthesis stage, the sintering process in the KNN lead-free ferroelectric ceramics is a crucial step to produce materials with high electromechanical properties. It has been found that a narrow sintering range exists (Y. Wang et al., 2007) where the materials experience considerable changes in the grain size, density, appearance of secondary phases, liquid phase, and then the piezoelectric and ferroelectric properties change as well. In the text below, are discussed some of the sintering methods used for the conformation of KNN ceramics. First, the conventional sintering (CS), then the hot pressing (HP) and finally the spark plasma sintering (SPS) are going to be described.
5.1. Conventional sintering
The method consists of pressing the powders in a uniaxial press or through cold isostatic pressing. Then, the green pellets are heat treated in a high temperature furnace. The sintering temperature depends upon the composition for pure KNN samples the temperature is set between 1020 and 1120°C. The method is simple and economic comparing with HP or SPS which will be described in the next sections. Most studies about KNN and related compositions use conventional sintering (Chang et al., 2007; Egerton & Dillon, 1959; Hao et al., 2009; Park et al., 2007; Saito & Takao, 2006; Y. Wang et al., 2007; Zuo et al., 2007), and just some papers report lead-free piezoceramics sintered by HP or SPS. In conventional sintering two steps are commonly used during the treatment, first the binder burn out at 400-500°C, and then the sintering at high temperatureproceeds. This high temperature stage is performed from 1 to ~ 12 hours. For instance sintering a Li doped KNN composition gave optimal results when the time was set at 8 h ( Wang et al., 2010 ), but it is common to use 2 h. It has been observed the influence of the heating rate over the properties, these rates are close to 4-5°C/min (Du et al., 2006).The fundamental objective to investigate these issues is to determine the effects on the grain growth and hence on the ferroelectric and piezoelectric properties. Most of the investigations try to search for sintering conditions that avoid or reduce at least, the loss of alkaline elements. Combining the ceramic method for the synthesis and the conventional sintering results in low density materials.For this reason, the HP and the SPS methods are being explored, mainly the later, for the improvement of density and the correspondingly enhancement in theelectromechanical performance of ceramics.
5.2. Hot pressing
This method has the advantage that pressure and temperature are simultaneously applied, being able to obtain a better densification. Nevertheless, the sintering temperatures are as high as in the conventional sintering.Furthermore, few data on electromechanical properties have been reported by means of this technique (Jaeger & Egerton, 1962). The piezoelectric properties have been improved considerably using this method, compared as those sintered conventionally.
5.3. Spark plasma sintering
The SPS technique is not new in the field of sintering, but its use was not exploited for sintering lead-free piezoelectric ceramics. Very recently it was applied for sintering KNN (K. Wang et al., 2008 ), and related compositions (Abe et al., 2007; Shen et al., 2010). The advantage of the SPS over CS or HP is that it requires lower temperatures and shorter times for producing ceramics with densities close to the theoretical values. Commonly, heating rates are around 100°C/min, so in few minutes the sintering temperature is achieved; as a result the sintering time is reduced by several hours. This is possible due to the heating mechanism. In this method, a very high electric current is passed through the sample and pressure is applied simultaneously, and liquid phase is generated rapidly which assist the densification, but for more details the reader is encouraged to revise some specialized publications on the subject (Hungría et al., 2009; Tokita, 1993). This sintering method allows reducing the loss of alkaline elements because of the low sintering temperature and short holding time; nevertheless, additional heat treatment is required to eliminate oxygen vacancies (Abe et al., 2007; Wang et al., 2007). In Fig. 3 the SEM images of KNLNT sintered samples by CS and SPS are shown (López-Juárez et al., 2011b), it is clearly observed the difference in densification (porosity). The difference in densification level affects directly the piezoelectric and dielectric properties.
6. Synthesis of K0.5Na0.5NbO3 and (K0.48Na0.52)0.96Li0.04Nb0.85Ta0.15O3 by spray drying
As already mentioned, the key problem with the synthesis of KNN is there are no stable niobium chemical reagents to use in sol-gel, Pechini or whatever the method employed. The only stable niobium compound is the oxide (Nb2O5). Then, the synthesis of KNN based ceramics has been reviewed in previous sections, emphasizing the chemical methods used until now. In this work a new approach is described as is reported elsewhere (López et al., 2010, 2011b). The spray drying method was employed to synthesize chemically homogeneous powders. For this purpose the chelation of niobium and/or tantalum is necessary. In our preparation methodit was possible to synthesize lead-free ferroelectric ceramics stabilizing niobium with an organic acid, by previously dissolving Nb2O5 and precipitating the corresponding hydrated oxide (López et al., 2010), this is also applicable to Ta2O5 because it behaves in a similar manner. Actually, tantalum is introduced into the KNN solid solution structure. The K0.5Na0.5NbO3 and (K0.48Na0.52)0.96Li0.04Nb0.85Ta0.15O3 compositions were synthesized. It was probed that the crystallization can be set at 800°C with a heating time of 1 hour. Finally, the microwave-hydrothermal method was tested for KNN synthesis, and interesting results are going to be released.
6.1. Characterization of the synthesized powders
In Fig. 4 the X-Ray diffraction patterns of the two compositions are shown. The most interesting feature is that the powders are chemically pure when calcined at 800°C for 1 h, irrespective of the composition. It is observed that the as sprayed powders are amorphous in both compositions. For the KNN powders, the subsequent heat treatment at 600ºC generates the formation of two phases; the K6Nb10O30 phase (JCPDS 70-5051) with tetragonal structure and the KNN perovskite phase with orthorhombic lattice.
When powders were calcined at 700ºC the amount of tetragonal phase diminishes considerably, this fact is noticed by the reduction in the Bragg reflections corresponding to the tetragonal phase, and at 750ºC only perovskite phase is observed. The calcination temperature and time are lowered compared with those required in the synthesis by the ceramic method. For the KNLNT composition (Fig. 4b), once the powders were thermally treated at 600°C several Bragg reflections appeared, corresponding to the tetragonal
secondary phase K3Li2Nb5O15 (JCPDS-ICDD 52-0157) and those expected for KNLNT phase were observed. The secondary phase diminish for the samples calcined at 750°C and at 800°C only reflections of the KNLNT phase remains. The TEM images of the calcined powders reveal the fine particle size with average grains < 0.3 μm (Fig. 5). In Fig. 5a the bright field and 5b the high resolution images of KNN powders are shown. The typical cubic shape of KNN is clearly seen (Jenko et al., 2005). The KNLNT crystalline powders are shown in Figs. 5c and 5d, a bright field (BF) image and the corresponding high resolution (HR) picture are observed, where it is shown that the addition of tantalum has inhibited the grain growth, as reported before (Saito & Takao, 2006) compared with KNN. In the high resolution image the coalescence between two nanocrystals is depicted with the crystalline planes well developed. The average grain size for KNN powders was 281 nm and 100 nm for KNLNT, the measurements were done over several bright field TEM images using the ImageJ software. The particle size achieved by the spray drying route is comparable with those results of sol-gel and Pechini method. The small grains contain high surface energy that is one of the driving forces for sintering. It is known that in addition to the surface energy, the pressure and chemical reactions would aid the sintering (Rahaman, 2006), the later being uncommon for this purpose.
The combination of pressure and heating at the same time in hot-pressing or spark plasma sintering, does not require necessarily very small particles in order to obtain high density materials, but for conventional sintering it is desirable to synthesize finer particles to get high densities in bulk ceramics.
6.2. Sintering, piezoelectric and ferroelectric properties of lead-free ceramics
The synthesis is only the first step in the processing of ferroelectric ceramics. Pressing and sintering are another two important issues for completing the whole process. Then, in the following paragraphs the sintering and the properties of the prepared ceramics are presented.
6.2.1. Sintering of KNN powders
The consolidation and sintering of ferroelectrics ceramics with KNN composition is described in our previous publication (López et al., 2011a). For a sort of clarity, here we are giving some more details. The calcined powders at 800°C for 1 h were pressed in a uniaxial press at 443 MPa. Then the pressed samples were placed into a high temperature furnace and sintered for 2 hours. The heating rate was set at 7°C/min, the sintering temperature was established at 1060-1120°C, that isthe ideal sintering treatment for which the highest piezoelectric properties were measured. The density was measured by the Archimedes method in distilled water.
In Fig. 6 the images of KNN sintered samples are shown. Evidently, with increasingofthe sintering temperature the grain size increases. But, first the density increases when passing from 1060°C to 1080°C, and then decreases at 1100 and 1120°C, this coincides with the SEM images, where considerable pores are seen in the sample sintered at 1060°C and diminished at 1080°C (Fig. 7b). The higher density was that of the sample sintered at 1080°C, 4.33 g/cm3 (96% of theoretical value, 4.51g/cm3 being the referencevalue). The low density of the samples sintered at 1100 and 1120°C are due to the formation of liquid phase and the considerable volatilization of alkaline elements (Jenko et al., 2005; López et al., 2011a; K. Wang et al., 2010 ).
6.2.2. Piezoelectric, dielectric and ferroelectric properties of KNN
For the piezoelectric properties evaluation, the measurements were done on the poled samples, also the dielectric constant and losses were acquired, the
The piezoelectric properties are also related with the remnant polarization (
In the high resolution image the atomic columns are observed, and some vacancies are highlighted with arrows that are seen as unfilled gaps. The image was taken in the  direction of the orthorhombic lattice, the typical hexagonal geometry of atomic columns is clearly distinguished.
The piezoelectric properties obtained for the sintered samples are summarized in table 1. As was stated above, the best properties are those for the sintered pellet at 1080°C. In table 2, the properties of KNN reported for several authors are shown. It can be seen that the properties of the ceramics processed by spray drying and conventionally sintered are comparable with those previously reported.
|Parameter||Sintering temperature (°C)|
|0.36||80||32||290(100 kHz)||4.24||2(100 kHz)||---||Egerton & Dillon, 1959|
|0.45||160||49||420(100 kHz)||---||1.4(100 kHz)||---||Jaeger & Egerton, 1962|
|0.32||107||---||264(1 kHz)||4.09||---||---||Maeda et al., 2010|
|0.40||120||---||500(1 kHz)||4.4||---||400||Du et al., 2006|
|0.39||70 – 90||45||400(1 kHz)||4.28||2.5 (1 kHz)||390||Ringgaard &|
|---||---||---||----||---||1.3 (10 kHz)||395||Singh et al., 2001|
|0.34||---||46.2||453(1 kHz)||---||35(1 kHz)||402||L. Liu et al., 2009|
|0.36||117||30||309(100 kHz)||4.33||1.6(100 kHz)||419||López et al., 2011a|
It is obvious the wide range of values of the piezoelectric properties, even when most authors use the conventional ceramic method for the production of ferroelectric ceramics. This remarks the sensitiveness of these materials to any small processing variation, the moisture sensitivity of alkaline carbonates, the calcination temperature, the heating time and, finally, the temperature at the sintering stage. All these steps considered together influence the poling process and then and final performance of the ceramics.
To conclude this section it should be mentioned the efforts to achieve the low temperature synthesis of KNN powders as was underlined at the hydrothermal synthesis section. This method requires heat treatment for a long time at low temperature (<300°C) if the conventional hydrothermal method is used. But recently, the microwave-hydrothermal technique it is being explored for the synthesis of some inorganic materials. Although, the influence of microwaves on the reaction system it is not well understood until now. In the case of potassium-sodium niobate, the synthesis was proved to proceed faster with the aid of microwaves. The sintered powders experienced extremely grain growth with grain size average > 60 μm where the ferroelectric domains were reveled easier. In Fig. 10 the ferroelectric domains are shown in the ceramics sintered at 1080°C for 4 hours in air. As it isobserved, the ferroelectric domains are large enough to be revealed by contrast using backscattered electrons (at 1 pA and 20kV), and in etched samples with hydrofluoric acid. The domain structure was found to be constituted mostly by 90° and 180° ferroelectric domains, for more details refer to the work by López et al.(López et al., 2011c).
6.2.3. Sintering of KNLNT
The synthesized powders by spray drying with (K0.48Na0.52)0.96Li0.04Nb0.85Ta0.15O3 composition were pressed and sintered at 1100-1150°C in air for 2 hours. The SEM pictures of these samples are shown in Fig. 11. The grain size was smaller comparing with the KNN composition. It is reported that the addition of Ta+5 into the KNN structure inhibits grain growth (Saito & Takao, 2006). When the sintering temperature was set at 1100°C, the grains grow inhomogeneously, but increasing the temperature to 1120 and 1130°C, these are bigger with the characteristic cubic shape, and for 1150°C, the grains grew even more because the faster mass transport rate. The densities and other piezoelectric parameters are shown on table 3. As it was observed for KNN ceramics, here the behavior of density and piezoelectric properties first increase and then fall for samples sintered at higher temperature. The factors which affect the densification of KNN pellets are also present for KNLNT composition. Evidently, the high temperature used for the sintering is because of the Ta+5 content, and the low concentration of Li+1 on the system, despite that, it is well known that lithium aids densification at lower temperatures as compared with KNN.
6.2.4. Piezoelectric, dielectric and ferroelectric properties of KNLNT
The KNLNT samples were processed and poled as reported before (López et al., 2010). In table 3, the properties obtained for the samples sintered at 1100 and 1150°C are also included. The values of piezoelectric properties increase with increasing sintering temperature, reaching maximum values for 1120°C, and then decrease for 1130 and 1150°C. In these materials is common to reach equilibrium between sintering temperature and piezoelectric properties. The temperature must be high enough to guarantee the diffusion of matter, eliminate pores and to promote grain growth, but not too high for avoiding the volatilization of alkaline elements and the formation of secondary phases, which degrades the piezoelectric properties. The presence of secondary phases, liquid phase or a high concentration of vacancies would result in incomplete poling because the leakage current leads to poor performance. Then the optimum sintering temperature of KNLNT ceramics was established at 1120°C. At this temperature the density,
|Parameter||Sintering temperature (°C)|
|(10−12 m2 N−1)||12.33||11.80||12.24||13.12|
|(10−12 m2 N−1)||-4.15||−2.786||-3.64||-4.271|
It has been demonstrated that the magnitude of the dielectric constant is affected by extrinsic variables as the porosity (Fang et al., 1993), i.e. the air trapped within the samples has a low
This is completely in agreement with the piezoelectric properties of the sintered ceramics. Probably, the most important issue is the crystal structure of the ceramics, if it is assumed that for KNLNT the polymorphic phase transition (PPT) is close to room temperature, and invoking the assumption that orthorhombic and tetragonal phases coexist at the PPT, then the polarization will be enhanced and the piezoelectric properties improved as well. This is evident when compared the properties found in KNN and KNLNT.
In table 4, the comparison of several compositions is presented. In the same wayas the results for pure KNN, the properties cover a wide range of values also for KNLNT and related compositions. It is observed that in compositions with BaTiO3
|0.95(Na0.5K0.5)NbO3-0.05CaTiO3||0.41||241||1316(10 kHz)||9.0(10 kHz)||306||Park et al., 2007|
|(Na0.5K0.5)0.97La0.01Nb0.95Ta0.05O3||0.37||119||815(10 kHz)||4.5(10 kHz)||340||Hao et al., 2009|
|(K0.44Na0.52Li0.04)(Nb0.84Ta0.10Sb0.06)O3||0.48||299||1865(1 kHz)||2.1(1 kHz)||265||Hagh et al., 2007|
|(K0.5Na0.5)0.096Li0.04Nb0.775Ta0.225O3||0.48||208||1146||< 3||320||Lin et al., 2007|
|(Na0.52K0.4375)(Nb0.9175Sb0.04)O3–0.0425LiTaO3||0.48||310||1644(10 kHz)||---||337||Fu et al., 2008|
|(K0.38Na0.52Li0.04)(Nb0.86Ta0.10Sb0.04) O2.97||0.37||195||1060(1 MHz)||2.8(1 MHz)||276||Rubio-Marcos et al., 2007|
|(Li0.04K0.44Na0.52)(Nb0.85Ta0.15)O3||0.38||200||---||---||---||Li et al., 2008|
|0.97Li0.06(Na0.5K0.5)0.94NbO3–0.03BaTiO3||0.32||128||800(1 kHz)||---||370||Kakimoto et al., 2010|
|0.42||209||1100(10 kHz)||2.6(10 kHz)||344||Zang et al., 2010|
|0.92(K0.5Na0.5)NbO3–0.08AgTaO3||0.41||183||683(10 kHz)||3.3(10 kHz)||356||Wang et al., 2010|
|(K0.48Na0.52)0.96Li0.04Nb0.85Ta0.15O3||0.41||186||465(10 kHz)||1.0(10 kHz)||354||López et al., 2010|
In the last few years several researches were performed in the lead-free ferroelectric materials for piezoelectric applications. These works were focused in the improvement of the piezoelectric properties by doping potassium-sodium niobate ceramics. The dopants are those of the A and B occupancy within the perovskite structure. Most of them shift the
In this work, the spray drying synthesis method was used to synthesize KNN and KNLNT ceramics. The obtained results pointed out that this method is a promising option for avoiding inhomogeneous distribution of cations within the ceramics, and the losses of alkaline elements. This was possible because the temperature and time at the calcination stage were reduced. The sintered ceramics shown good piezoelectric and ferroelectric properties, i.e. high kp, low tanδ and ε, and moderate EC and Pr. In the case of KNLNT the ideal sintering temperature, depends greatly upon the doping elements. In the KNLNT the improvement of the piezoelectric properties was attributed to the polymorphic phase transition close to room temperature.
The authors want to thank to Dr. Fernando Rubio and Prof. José F. Fernández (ICV-CSIC)for the evaluation of the d33 constant. Special thanks to Omar Novelo-Peralta (Instituto de Investigaciones en Materiales-Universidad Nacional Autónoma de México [IIM-UNAM]) and Ariosto Medina (Instituto de Investigaciones Metalúrgicas-Universidad Michoacana de San Nicolás de Hidalgo) for the SEM and TEM images, respectively. The authors are indebted to Dr. M.P. Cruz(CNyN-UNAM) for the access to the Radiant workstation for ferroelectric loops measurements. Finally, R. López-Juárez wants to acknowledge to CONACyT-México and to IIM-UNAM for the PhD scholarships.
Abe J. Kobune M. Kitada K. Yazawa T. 2007Effects of Spark-Plasma Sintering on the Piezoelectric Properties of High-Density (1-x)(Na0.5K0.5)NbO3-xLiTaO3 Ceramics.
Ahn C. W. Park C. S. Choi C. H. Nahm S. Yoo M. J. Lee H. G. Priya S. 2009Sintering behavior of lead-free (K,Na)NbO3-based piezoelectric ceramics
Alemany C. Gónzalez A. M. Pardo L. Jiménez B. Carmona F. Mendiola J. (1995 1995Automatic determination of complex constants of piezoelectric lossy materials in the radial mode.
Buhrer C. F. 1962Some properties of bismuth perovskites:
Chang R. C. Chu S. Y. Lin Y. F. Hong C. S. Wong Y. P. 2007An investigation of (Na0.5K0.5)NbO3-CaTiO3 based lead-free ceramics and surface acoustic wave devices.
Chen K. Xu G. Yang D. Wang X. (2007 2007Dielectric and Piezoelectric Properties of Lead-Free 0.95(K0.5Na0.5)NbO3-0.05LiNbO3 Crystals Grown by the Bridgman Method.
Chowdhury A. Bould J. Zhang Y. James C. Milne S. J. (2010 2010Nano-powders of Na0.5K0.5NbO3 made by a sol-gel method.
Chowdhury A. O’Callaghan S. Skidmore T. A. James C. Milne S. J. (2009 2009Nanopowders of Na0.5K0.5NbO3 Prepared by the Pechini Method.
Du H. Li Z. Tang F. Qu S. Pei Z. Zhou W. 2006Preparation and piezoelectric properties of (K0.5Na0.5)NbO3 lead-free piezoelectric ceramics with pressure-less sintering.
Egerton L. Dillon D. M. (1959 1959Piezoelectric and Dielectric Properties of Ceramics in the System Potassium Sodium Niobate.
European commission. 2008Recast of the WEEE and RoHS Derectives proposed, In:
Fang T. T. Hsieh H. L. . Shiau F. S. (1993 1993Effects of Pore Morphology and Grain Size on the Dielectric Properties and Tetragonal-Cubic Phase Transition of High-Purity Barium Titanate.
Fu J. Zuo R. Wu Y. Xu Z. Li L. (2008 2008Phase Transition and Electrical Properties of Li-and Ta-Substituted (Na0.52K0.48)(Nb0.96Sb0.04)O3 Piezoelectric Ceramics.
Gao D. Kwok K. W. Lin D. Chan H. L. W. 2009Microstructure, electrical properties of CeO2-doped (K0.5Na0.5)NbO3 lead-free piezoelectric ceramics.
0935-9648 3 20 551 555 Guillemet-Fritsch, S.; Valdez-Nava, Z.; Tenailleau, C.; Lebey, T.; Durand, B. & Chane-Ching, J.Y. (2008). Colossal permittivity in ultrafine grain size BaTiO3-x and Ba0.95La0.05TiO3-x materials. Adv. Mater. Vol. 20, No. 3, (Feb 2008), pp. 551-555, ISSN 0935-9648
Guo Y. Kakimoto K. Ohsato H. 2004Phase transitional behavior and piezoelectric properties of (Na0.5K0.5)NbO3-LiNbO3 ceramics.
Haertling G. H. 1999Ferroelectric ceramics: History and technology.
Hagh N. M. Jadidian B. Safari A. 2007Property-processing relationship in lead-free (K, Na, Li)NbO3-solid solution system.
Hagh N. M. Kerman K. Jadidian B. Safari A. (2009 2009Dielectric and piezoelectric properties of Cu2+-doped alkali niobates.
Hao J. Xu Z. Chu R. Li W. Li G. Yin Q. 2009Relaxor behavior and dielectric properties of (La, Ta)-modified (K0.5Na0.5)NbO3 lead-free ceramics.
Hao J. Wang X. Chen R. Li L. 2005Synthesis of (Bi0.5Na0.5)TiO3 nanocrystalline powders by stearic acid gel method.
Hoshina T. Takizawa K. Li J. Kasama T. Kakemoto H. Tsurumi T. (2008 2008Domain Size Effect on Dielectric Properties of Barium Titanate Ceramics.
Hungría T. Galy J. Castro A. 2009Spark Plasma Sintering as a Useful Technique to the Nanostructuration of Piezo-Ferroelectric Materials.
Jaeger R. E. Egerton L. (1962 1962Hot Pressing of Potassium-Sodium Niobates.
Jaffe B. Cook W. R. Jaffe H. (1971 1971
Jaffe H. 1958Piezoelectric Ceramics.
Jenko D. Benčan A. Malič B. Holc J. Kosec M. 2005Electron Microscopy Studies of Potassium Sodium Niobate Ceramics.
Jiang M. Liu X. Chen G. Zhou C. 2009Dielectric and piezoelectric properties of LiSbO3 doped 0.995 K0.5Na0.5NbO3-0.005BiFeO3 piezoelectric ceramics.
Jing X. Li Y. Yin Q. (2003 2003Hydrothermal synthesis of Na0.5Bi0.5TiO3 fine powders.
Kakimoto K. Ando K. Ohsato H. 2010Grain size control of lead-free Li0.06(Na0.5K0.5)0.94NbO3 piezoelectric ceramics by Ba and Ti doping.
Kizaki Y. Noguchi Y. Miyayama M. 2007Defect Control for superior Properties in Single Crystals.
Li H. D. Feng C. D. Yao W. L. 2004Some effects of different additives on dielectric and piezoelectric properties of (Bi1/2Na1/2)TiO3-BaTiO3 morphotropic phase boundary composition.
Li J. F. Zhen Y. Zhang B. P. Zhang L. M. Wang K. 2008Normal sintering of (K, Na)NbO3-based lead-free piezoelectric ceramics.
Lin D. Kwok K. W. Chan H. L. W. (2007 2007Microstructure, phase transition, and electrical properties of (K0.5Na0.5)1−xLix(Nb1−yTay)O3 lead-free piezoelectric ceramics.
Lin D. M. Xiao D. Q. Zhu J. G. Yu P. 2006Piezoelectric and ferroelectric properties of [Bi0.5(Na1-x-yKxLiy)(0.5)]TiO3 lead-free piezoelectric ceramics.
Liu L. Fan H. Fang L. Chen X. Dammak H. Thi M. P. (2009 2009Effects of Na/K evaporation on electrical properties and intrinsic defects in Na0.5K0.5NbO3 ceramics.
Liu N. Wang K. Li J. F. Liu Z. (2009 2009Hydrothermal Synthesis and Spark Plasma Sintering of (K,Na)NbO3 Lead-Free Piezoceramics.
López R. González F. Villafuerte-Castrejón M. E. (2010 2010Structural and electrical characterization of (K0.48Na0.52)0.96Li0.04Nb0.85Ta0.15O3 synthesized by spray drying.
López R. González F. Cruz M. P. Villafuerte-Castrejon M. E. (2011a 2011aPiezoelectric and ferroelectric properties of K0.5Na0.5NbO3 ceramics synthesized by spray drying method.
Villafuerte-Castrejón, M.E. ( López-Juárez R. González-García F. Zárate-Medina J. Escalona-González R. Díaz la Torre. 2011bPiezoelectric properties of Li-Ta co-doped potassium-sodium niobate ceramics prepared by spark plasma and conventional sintering.
Ferroelectric domain structure of lead-free potassium-sodium niobate ceramics. López-Juárez R. Novelo-Peralta O. González-García F. Rubio-Marcos F. Villafuerte-Castrejón M. E.
Ma Y. J. Cho J. H. Lee Y. H. Kim B. I. 2006Hydrothermal synthesis of (Bi1/2Na1/2)TiO3 piezoelectric ceramics.
Maeda T. Takiguchi N. Ishikawa M. Hemsel T. Morita T. 2010K,Na)NbO3 lead-free piezoelectric ceramics synthesized from hydrothermal powders.
Merz W. J. 1949The electric and optical behavior of BaTiO3 single-domain crystals.
Morrison F. D. Sinclair D. C. West A. R. (1999 1999Electrical and structural characteristics of lanthanum-doped barium titanate ceramics.
Nagata H. Takenaka T. 2001Additive effects on electrical properties of (Bi1/2Na1/2)TiO3 ferroelectric ceramics.
Nagata H. Yoshida M. Makiuchi Y. Takenaka T. 2003Large piezoelectric constant and high curie temperature of lead-free piezoelectric ceramic ternary system based on bismuth sodium titanate-bismuth potassium titanate-barium titanate near the morphotropic phase boundary.
Noheda B. Cox D. E. Shirane G. Gonzalo J. A. Cross L. E. Park S. E. 1999A monoclinic ferroelectric phase in the Pb(Zr1-xTix)O3 solid solution.
Park H. Y. Cho K. H. Paik D. S. Nahm S. 2007Microstructure and piezoelectric properties of lead-free (1-x)(Na0.5K0.5)NbO3-xCaTiO3 ceramics.
Pardo L. García A. Brebøl K. Curecheriu L. P. Mitoseriu L. Mercadelli E. Galassi C. 2010Piezoelectric characterization of lead-free ferroelectric ceramics.
Rahaman M. N. 2006
Ringgaard E. Wurlitzer T. 2005Lead-free piezoceramics based on alkali niobates.
Rojac T. Bencan A. Ursic H. Malic B. Kosec M. 2008Synthesis of a Li- and Ta-modified (K,Na)NbO3 solid solution by mechanochemical activation.
Rubio-Marcos F. Ochoa P. Fernandez J. F. 2007Sintering and properties of lead-free (K,Na,Li)(Nb,Ta,Sb)O3 ceramics.
High Performance Lead-free Piezoelectric Ceramics in the (K,Na)NbO3-LiTaO3 Solid Solution System. Saito Y. Takao H.
Saito Y. Takao H. Tani T. Nonoyama T. Takatori K. Homma T. Nagaya T. Nakamura M. (2004 2004Lead-free piezoceramics.
Scott F. J. 2007Applications of modern ferroelectrics.
Scott F. J. 2008Ferroelectrics go bananas.
Shen Z. Y. Li J. F. Wang K. Xu S. Jiang W. Deng Q. (2010 2010Electrical and Mechanical Properties of Fine-Grained Li/Ta-Modified (Na,K)NbO3-Based Piezoceramics Prepared by Spark Plasma Sintering.
Dielectric properties and phase transitions of NaNbO3 and (Na,K)NbO3. Shirane G. Newnham R. Pepinsky R.
Shiratori Y. Magrez A. Pithan C. 2005Particle size effect on the crystal structure symmetry of K0.5Na0.5NbO3.
Singh K. Lingwal V. Bhatt S. C. Panwar N. S. Semwal B. S. 2001Dielectric properties of potassium sodium niobate mixed system.
Smolenskii G. A. Isupov V. A. Agranovskaya A. I. Krainik N. N. (1961 1961New ferroelectrics of complex composition.4.
Sun C. X. Chen J. Deng J. Li L. Yu R. Qiao L. Liu G. 2007Hydrothermal Synthesis of Single Crystalline (K,Na)NbO3 Powders.
Takenaka T. . Sakata K. Toda K. 1990Piezoelectric properties of (Bi1/2Na1/2)TiO3-based ceramics.
Takenaka T. Nagata H. Hiruma Y. (2008 2008Current Developments and Prospective of Lead-Free Piezoelectric Ceramics.
Tokita M. (1993 1993Trends in advanced SPS Spark Plasma Sintering Systems and Technology.
von Hippel. A. Breckenridge R. G. Chesley F. G. Tisza L. 1946High Dielectric Constant Ceramics.
Wang K. Li J. F. (2010 Low 2010Low-Temperature Sintering of Li-Modified (K, Na)NbO3 Lead-Free Ceramics: Sintering Behavior, Microstructure, and Electrical Properties.
Wang K. Zhang B. P. Li J. F. Zhang L. M. 2008Lead-free Na0.5K0.5NbO3 piezoelectric ceramics fabricated by spark plasma sintering: Annealing effect on electrical properties.
Wang Y. Damjanovic D. Klein N. Hollenstein E. Setter N. (2007 2007Compositional Inhomogeneity in Li- and Ta-Modified (K, Na)NbO3 Ceramics.
Wang Y. Qibin L. Zhao F. 2010Phase transition behavior and electrical properties of [(K0.50Na0.50)1−xAgx](Nb1−xTax)O3 lead-free ceramics.
Wang Y. Wu J. Xiao D. Zhu J. Yu P. Wu L. Li X. 2008Piezoelectric properties of (Li, Ag) modified (Na0.5K0.50)NbO3 lead-free ceramics with high Curie temperature.
West A. R. 2006Inorganic functional materials: Optimization of properties by structural and compositional control.
Wul B. M. Goldman I. M. (1945 1945Dielectric Constants of Titanates of Metals of the Second Group.
Yang W. Jin D. Wang T. Cheng J. 2010Effect of oxide dopants on the structure and electrical properties of (Na0.5K0.5)NbO3-LiSbO3 lead-free piezoelectric ceramics.
Yao Z. H. Liu H. X. Chen L. Cao M. H. 2009Morphotropic phase boundary and piezoelectric properties of (Bi0.5Na0.5)(1-x)(Bi0.5K0.5)(x)TiO3-0.03(Na0.5K0.5)NbO3 ferroelectric ceramics.
Yin Q. Yuan S. Dong Q. Tian C. 2010Effect of CuO and MnO2 doping on electrical properties of 0.92(K0.48Na0.54)NbO3-0.08LiNbO3 under low-temperature sintering.
Yoon S. Baik S. Kim M. G. Shin N. Kim I. 2007Synthesis of tetragonal barium titanate nanoparticles via alkoxide-hydroxide sol-precipitation: Effect of water addition.
Yu J. Paradis P. F. Ishikawa T. Yoda S. Saita Y. Itoh M. Kano F. (2004 2004Giant Dielectric Constant of Hexagonal BaTiO3 Crystal Grown by Containerless Processing.
Zang G. Z. Yi X. J. Xu Z. J. Pu X. P. Fu P. Zhao L. M. 2010Lead-free (K0.5Na0.5)0.95(LiSb)0.05Nb0.95O3-BaTiO3 Piezoceramics.
Zhang S. T. Kounga A. B. Aulbach E. Granzow T. Jo W. Kleebe H. J. Rodel J. (2008 2008Lead-free piezoceramics with giant strain in the system Bi0.5Na0.5TiO3-BaTiO3-K0.5Na0.5NbO3. I. Structure and room temperature properties.
Zhao W. Zhou H. P. Yan Y. K. Liu D. Liu S. S. 2007Influence of different dopants on the piezoelectric properties of the Na1/2Bi1/2TiO3-BaTiO3- lead-free ceramics,
Zhou C. Liu X. Li W. Yuan C. 2009Dielectric and piezoelectric properties of Y2O3 doped (Bi0.5Na0.5)(0.94)Ba0.06TiO3 lead-free piezoelectric ceramics.
Zhou Y. Yu J. Guo M. Zhang M. 2010Microwave Hydrothermal Synthesis and Piezoelectric Properties Investigation of K0.5Na0.5NbO3 Lead-Free Ceramics.
Zuo R. Ye C. Fang X. (2007 2007Dielectric and Piezoelectric Properties of Lead Free Na0.5K0.5NbO3-BiScO3 Ceramics.